Characterization of activated carbon produced from coffee residues by chemical and physical activation
JAVIER SNCHEZ AZNARKTH Chemical Science and Engineering
Master Thesis in Chemical Engineering Stockholm, Sweden, March 2011
List of figuresPART 1 Fig 1.1 Representation of the structure of activated carbons (H. Fritzst Oeckli 1990)(47).7 Fig 1.2 The six isotherm types according to IUPAC...8 Fig 1.3 Representation of the three types of pores according to the IUPAC.....14 Fig 1.4 Texture of dust activated carbon...19 Fig 1.5 Texture of granular activated carbon.19 Fig 1.6 Structure of a coffee bean..23 PART 2 Fig 2.1 Furnace employed for carbonization.31 Fig 2.2 Magnetic stirrer during HCL washing..32 Fig 2.3 Steam activation system33 Fig 2.4 ASAP instrument...34 PART 3 Fig 3.1 Results of yields for 30%, 40% and 50% samples by chemical activation at different temperatures....38 Fig 3. 2. Results of yields for samples activated by steam at different temperatures39 Fig 3.3 Results of volatile and ash content by chemical and steam activation..40 Fig 3.4 Results of BET surface area (m2/g)...42 Fig 3. 5 Isotherm of the sample CA_3_500...44 Fig 3.6 Isotherm of the sample CA_3_600....44 Fig 3.7 Isotherm of the sample CA_3_700....44 Fig 3.8 Isotherm of the sample CA_4_500....45 Fig 3.9 Isotherm of the sample CA_4_600....45 Fig 3.10 Isotherm of the sample CA_4_700......45 Fig 3.11 Isotherm of the sample CA_5_500......46 Fig 3.12 Isotherm of the sample CA_5_600......46 Fig 3.13 Isotherm of the sample CA_5_700......46
Fig 3.14 Isotherm of the sample TA_600......47 Fig 3.15 Isotherm of the sample TA_700..........47 Fig 3.16 Isotherm of the sample TA_800......47 Fig 3.17 Total pore volume and micropore volume for both activations..48 Fig 3.18 Results of total pore volume and BET surface area....50
List of tablesPART 1 Table 1.1 Characteristics of activated carbons..12 PART 2 Table 2.1 List of samples...30 PART3 Table 3.1 Results of yield (%), burn off (%) and chemical recovery...36 Table 3.2 Characteristics of common starting materials employed as activated carbon precursor (Manocha,2003)37 Table 3.3 Results of total pore volume, micropore volume, pore diameter and BET surface area of activated carbons with the concentration agent and temperature of activation..48
PART 1 Activated carbon1.1 IntroductionNowadays, there has been an increasing environmental concern around the world about emissions. Pollutants are constantly discharged to the environment water, soils and airand do also generate a lot of residues. Since years ago, there has been research going on to give value to wastes that had no value. In that sense the interest in utilization of several wastes has awaken the interest for the development of new processes where the production of adsorbents are gaining strength. Therefore, all-inexpensive residues with high carbon and low inorganic content can be considered as starting materials for the production of activated carbon, one of the most known and used adsorbent (1). That is why activated carbon produced from coffee residues could be used as efficient adsorbent with a lot of uses. That specific residue could be treated appropriately to obtain activated carbons, and so far, there are few studies (2-5) about its use as raw material for its preparation. The aim of this study is to evaluate the possibility of using this waste to obtain activated carbon. The production could be of great interest because the coffee consumption was around 8,2 kg per capita per year in Sweden in 2008 according to the International Coffee Organization (ICO) (http://www.ico.org/historical.asp). Activated carbon is largely used as versatile adsorbent with so many applications. Purification of water, air and many chemicals and natural products and its also widely used for adsorption and removal of pollutants from gaseous and liquid phases. It has several applications in medical, industrial and pharmaceutical processes.
1.2. Characterization of activated carbons1.2.1 Definition Activated carbon has been explained in different ways by several authors. Marsh (1989) defined activated carbon as porous carbon, which have been treated by oxidizing gases during or after carbonization in order to increase porosity. Norlia Baharun (1999) defined activated carbon as an organic material constituted basically by a graphitic structure. While according to Benaddi (2000) stated that activated carbon is predominantly an adsorbent with a large internal pore volume and surface are. Activated carbon can also be defined as any porous material formed in the major part of carbon and characterized by a well-developed porosity (6). Activated carbon is the generic term used to describe a family of amorphous carbonaceous adsorbents with a highly crystalline form and well developed internal pore structure. In general terms, one can differentiate two types of carbon: graphitizable and non graphitizable. Carbon is converted into graphite when it is burned to 3000C in an inert atmosphere. Activated carbons belong to the second group non-graphitizable carbonand are prepared from rich carbon materials that do not pass through a fluid phase during carbonization. A wide variety of commercial activated carbon products are available showing different characteristics depending on the starting material and activation method used in their production. According to R.C. Bansal et al (7) wood, coal, lignite, coconut shell and peat are the most important raw materials for the production of activated carbons, although other materials such as synthetic polymers or petroleum residues can also be used. Coffee wastes are one of the lignocellulosic residues generated in large quantities all over the world because coffee is the second largest traded commodity in the world, after petroleum.
Part 1 1.2.2 Characteristics of activated carbons 126.96.36.199 Adsorption process Adsorption is a physicochemical phenomenon in which a solid, called adsorbent, retain in the walls a certain kind of molecules, called adsorbates, that are contained in a gas or liquid. Hence it is a separation and concentration process of one or more compounds of a system on a solid or liquid surface. The most employed adsorbents are silica, some synthetic resins and activated carbons. Factors to be taken into consideration in an adsorption process regarding to the adsorbent adsorbate are the following: Specific surface and porosity of the solid Particle size Pore size, structure and distribution. Affinity of the adsorbate, depending of the chemical properties of the adsorbent surface. Partial pressure or concentration of the adsorbate in the fluid phase, where may be equilibrium established between the adsorbate concentration in the solution and the mass adsorbed per mass unit of the adsorbent using i.e. the Freundlich equation. There can be three types of adsorption attributed to the adsorbent-adsorbate attraction is electrical, Van der Waals or chemical. The first type is commonly called ion exchange because the ions of a substance are concentrated on the surface as a result of an electrostatic attraction. The Van der Waals adsorption also known as physical adsorption and takes place when the molecule is bound into the interphase usually at low temperatures. Most of organic compounds that are in water are adsorbed with activated carbons for this type of adsorption. The chemical adsorption is a reaction between the adsorbate and the adsorbent due to their chemistry and is characterized for being strong in the active point of the adsorbent.
Activated carbon In an adsorption process it is common to have a combination of all the three types. Actually, sometimes it is not easy to differentiate between a physical and chemical adsorption. The union between the adsorbates in the surface of the carbon is mostly caused by the Van der Waals forces, which means, that the activated carbon of apolar nature, will adsorb all the apolar substances depending on the affinity of the chemical surface properties. However, when there are mixtures of gases or substances with different affinity, the concentration of one of the substances will increase in the activated carbon surface, decreasing it in the mixture, until the adsorption-desorption equilibrium is achieved. In that sense, the process studied for evaluating an activated carbon is a term that explains the adhesion of ions, dissolved solids and all kind of molecules of gas and liquid including biomolecules to a solid surface. That process is explained by the force field created between the surface of the solid where the molecules fill in, the adsorption potentials are enhanced in micropores due to the overlap of the fields from the opposite pore walls and interactions between the adsorbed molecules. Adsorption is a superficial phenomenon, as high surface area the active carbon could achieve means that higher adsorptive capacity it will have. The surface is an important characteristic of the activated carbon and their typical range is around 500-1000m2/g (8). Besides achieving a high surface, it is also important to know the pore size distribution. The next picture is a representation of the structure of an activated carbon.
Fig 1.1 Representation of the structure of activated carbons (H. Fritzst Oeckli 1990) (47)
Adsorption is usually described through isotherms, which explains the relation of the amount of adsorbate on the adsorbent as a function of its pressure -gas- or concentration liquid- at constant temperature. In other words, there is the connection between relative vapour pressure and amount of adsorbed gas at a constant temperature. Actually, one can get useful information from isotherms about the adsorption volume, por